We follow the bouncing ball from the lab to the court.
By Rod Cross and Crawford Lindsey
Various tennis ball types are designed differently, manufactured differently, and perform differently. We set out to measure these differences using 26 different kinds of balls from eight manufacturers.
We tested only one can from each manufacturer. Was that can representative of all cans? Who knows? Would balls from 100 cans test the same relative to each other? Again, who knows? Were some balls fresh from the factory and others months old? What we do know is that our sample was probably just as good as any player’s “sample” when he goes to the store. Chances are that we got an average slice of reality, but we warn against making any absolute generalizations about specific ball types based on this limited data. What you can take away from the data are commonalities about the universe of balls. And these are interesting indeed.
All balls must meet ITF regulations in order to be approved for tournament play. Balls are subjected to strict testing procedures to determine whether they fall into the approved range of specifications for any given property of the ball. These tests include weight, size, rebound, and deformation. The acceptable ranges for the standard type 2 (medium speed) ball are as follows:
|Mass||1.975-2.095 ounces||56-59.4 grams|
|Size||2.575-2.700 inches||6.541-6.858 cm|
|Bounce||53-58 inches||135-147 cm|
|Forward deformation||0.220-0.290 inches||0.559-0.737 cm|
|Return deformation||0.315-0.425 inches||0.800-1.080 cm|
Together, these properties will determine how the ball bounces and feels on your racquet.
We performed the ITF tests plus a durability test. After the durability test, we put the used balls through the same tests again. The durability test involved firing each ball 30 times at high speed and oblique angle onto a cutout slab of hardcourt. The ball hit the fence and was returned to the ball machine via one bounce on the tennis court. In this way, we were able to measure new and used ball mass, diameter, bounce, and deformation.
One caveat is necessary. Although we performed all the ITF tests, they were not performed at the required temperature of 68 degrees F. An air-conditioning glitch necessitated that tests were performed at 73 degrees F. So the tests were not valid “pass/fail” tests, but they were accurate indications of the difference between balls. In any case, balls bounce a lot higher on a hot day than they do on a cold day, so a complete performance test should really be done at several different temperatures.
Due to time constraints, we did complete “used-ball” tests on only one ball from each can. We did “new-ball” tests on all three balls in each can.
Mass and Mass Loss
The range of all masses was between 54.66 and 59.04 grams. Three balls were below ITF specifications. The average mass of all three balls per can ranged from 55.25 to 58.90 grams.
The weight variance for all three balls within a can ranged from .04 to .58 grams.
After durability testing, balls lost between .34 and .94 grams. The photo shows a ball next to .22 grams of fuzz. Some balls lost four to five times that much fuzz!
The ITF approval is only a pass/fail test and does not measure the actual diameters. For the test, the ball in all orientations must be small enough to slip through the large hole and too large to drop through the small hole (see photo). We additionally measured the diameter of the largest of three perpendicular axes. Using a smooth vise, we measured the width of the vise gap that allowed the ball to drop when aligned along its widest axis. (Most balls were not absolutely round.)
The interesting observation is that the ball changes shape a little bit each time it is squashed, or in other words, after each hit. This was especially obvious after removing balls from the compression tester, but this is a slow compression (not like racquet impact) and the rubber has time to deform more.
Diameter variance within a can for all three balls ranged from 0.01 to 1.27 mm.
Under our test conditions of 73 degrees, balls dropped from 100 inches onto a granite surface bounced between 52.93 and 58.43 inches. The ITF requirements are for a bounce between 53 and 58 inches at 69 degrees.
Surprisingly, most balls bounced higher after the durability test than before — some more than 1.5% higher.
Standard ITF deformation (i.e., compression) tests were performed on all new balls. This involved (1) compressing each ball three times by 1 inch along all three axes to make sure the ball was round before testing it, (2) compressing the ball with a load of 18 pounds to measure the “forward deformation,” (3) increasing the load until the ball compressed 1 inch, and (4) decreasing the load back to 18 pounds to measure the “return deformation.” These steps were repeated for all three axes and the averages of each measurement were calculated.
These are static (not dynamic) stiffness tests. Consequently, it does not necessarily follow that a statically measured softer or stiffer ball will also be relatively softer or stiffer on racquet impact or that it will bounce higher or lower when it bounces off the court. In some respects, step 3 is more important than steps 2 or 4. Surprisingly, there is no ITF rule about the force required to compress a ball by 1 inch. A ball hit firmly compresses by around 1 inch. The compressions at steps 2 and 4 are only about 0.25 to 0.4 inch, which is about the same compression as a player achieves by squeezing the ball by hand. The ITF legislated “forward/return” deformation data is meaningless to most people, so we converted it to a simple stiffness calculation in terms of pounds necessary to compress the ball 1 inch.
Stiffness variance within a can for all three balls ranged from 0 to 10.53 lb/in with an average variance for all balls and brands of 2.63 lb/in.
Some very interesting and surprising observations arise from the results of these tests. Some of these are:
- Balls may bounce higher after use.
- Balls become softer with use.
- Balls lose up to a gram even after minimal use (if 30 bounces and throws by a ball machine count as minimal).
- Each ball in a can is different in weight, diameter, and bounce.
- Each can from the same manufacturer can be different.
- Balls bounce differently on different axes.
- Balls are not spherical.
- Balls change shape during play.
- Balls bounce up to 5 inches different between brands.
- Some balls/cans off the shelf may not be legal.
- Bounce depends on days out of the can, use, and temperature.
- Fuzz happens early in ball wear and then sheared off (this process might have been exaggerated with the ball machine).
So, differences abound. Seemingly, no two tennis balls, like no two fingerprints, are the same. No one can actually prove that. So far, all 40 million fingerprints held by the FBI are different, but the next one might well be an identical copy of number 12,583,912. Similarly, no one can prove that all tennis balls are different. So far, all 26 balls we tested were different, but it is possible that we might find two balls one day that are the same.
Regular and Extra Duty Balls
What is the difference? Regular duty felt is composed of a combination of slightly more wool than nylon fibers woven onto a cotton backing. As a rule, regular duty balls are designed for soft surfaces such as grass, carpet, and clay. These balls have a tighter weave, shorter nap, and thus play a little livelier and quicker due to less air friction and drag. The tighter weave is more clay, dirt, and moisture resistant; indoors, it leaves less fluff cleanup on the court and it inhibits fluffing due to static electricity.
Extra duty balls are designed for hard surfaces such as asphalt, concrete, and other outdoor hardcourts. Extra duty felt has a higher nylon content, resulting in a looser weave. Nylon does not weave as tightly as wool because it is a much smoother fiber. This causes the nylon to move around and fluff. A fluffy ball moves a bit slower through the air. Nylon is more resistant to abrasion than wool, but on an abrasive, hardcourt surface the fluff tends to be cut off as it forms.
Thus, if you use a regular duty ball on a hard court, it will fluff because the wool is not good against abrasion. It will also sheer more quickly. If you use an extra duty ball on grass or clay, it will pick up dirt in the loose weave and become heavier. If the ball does get fluffed up (from both the court and a lot of spin shots), it will tend to stay fluffy because there is not as much abrasion to shear it off. So if you use the wrong ball for the surface, you get either a prematurely bald ball or a poorly performing hairy one.
As a rule of thumb, a ball felt for your dog to chase in the back yard might be 100 percent unwoven Dacron or acrylic. An inexpensive mass merchandise ball might have a felt that is 15 percent wool, and a performance ball will be woven with about 50-60 percent wool, with extra duty types having more nylon.
TI magazine search
TI magazine articles
- Our Serve: Re-Evaluating What We Do
- Industry News
- Court Construction: Making Dreams a Reality
- Racquet Tech: Following Directions
- Retailing Tip: There Are Still Only Three Ways To Grow Your Retail Biz!
- Apparel Retailing: Clothes Calls
- Distinguished Facility-of-the-Year Awards: Residential Development
- Community Tennis: Local Heroes
- String Playtest: Pacific Poly Force Black Series 1.20
- Your Serve: The Perfect Storm